• date post

23-Mar-2022
• Category

## Documents

• view

0

0

Embed Size (px)

### Transcript of QUASI-STATIC AND DYNAMIC COMPACTION OF POROUS

1Yehuda Partom
12 March 2010Yehuda Partom2
Hydro-code Implementation
12 March 2010Yehuda Partom3
Herrmann’s EOS EOS for porous solids goes back to Herrmann [1].
He assumed that:
Herrmann’s assumption Pm
=αP needs to be checked on the mesoscale, but we adopt it anyway.
To complete the EOS one needs a relation α(P). In his well known Pα
model Herrmann assumes a P(α) polynomial, to be calibrated from tests. Part of what follows is about choosing or calculating an α(P) (or φ(P), φ=1-1/α) relation.
12 March 2010Yehuda Partom4
Instantaneous Pore Collapse This is a popular model and has many names.
It assumes that for P=0+: φ(=porosity)=0, or α=1, and: Vm
=V, Pm
=P, Em
=E.
( ) ( )( )
( ) ( )( )
+=
The Hugoniot curve of the porous material, obtained by eliminating E from the EOS and the energy equation: is:( )VVPE 02
1 −=
( ) ( ) ( )VVV
12 March 2010Yehuda Partom5
It is well known that for high porosities (>40%) the Hugoniot curves extend to the right of V=Vm0
. Using the above equation in this case means, that we rely on extrapolating the Hugoniot curve into the tension regime.
Instead we use the axis P=0 as the reference curve. We get:
( ) 0m
0m
0m
p
Γ +=
β ==
l
l
Implementing this instantaneous pore collapse model into a hydro-code we find that by using the axis as the reference curve for V>Vm0
we get much less noise at the shock level.
12 March 2010Yehuda Partom6
Many times details of the pore collapse process are of interest.
We then use gradual pore collapse models.
When φ(P) is known or assumed, we can use Herrmann’s EOS directly.
Two examples:
(φ):
2. Spherical shell plastic pore collapse (see later):
We introduce δ
goes to zero.
12 March 2010Yehuda Partom7
The pore collapse curve is also the elastic limit in compression.
For an initial porosity φ0
, pressure increases elastically without change of porosity until the pore collapse curve is reached.
The elastic limit is given by: ( )
( )

−+=
PP
where the degraded modulii are given by Eshelby’s solution as:
m 2 1
m 4 3
=
The Hugoniot curve centered at the elastic limit is then given by:
12 March 2010Yehuda Partom8
PVEE
VVPPEE
In Figs. 1 and 2 we compare two calculated Hugoniot curves for porous SS with 20% initial porosity. 1. Gradual pore collapse. 2. Instantaneous pore collapse.
Fig. 1
P re
ss ur
e (G
P a)
Instantaneous pore collapse Gradual pore collapse
S ho
ck v
el oc
ity (k
m /s
∂ ∂
V EdP
dP dE
P EdE
dP dE
P E
V EqP
dV dP
∂ ∂
( )
12 March 2010Yehuda Partom11
We get two first order ODEs to integrate for each computational cell at the EOS/energy stage of each time step: dP/dV= and dφ/dV= . Vi
and Vf
are given, and we assume that V varies linearly between them.
Fig. 3 is a history plot of a planar impact calculation where a 20 GPa shock enters a 20% porous SS sample. We show P(V) and compare it to the Hugoniot curve in Fig. 1.
0
5
10
15
20
25
Hydro-code Hugoniot
P re
ss ur
e (G
P a)
12 March 2010Yehuda Partom12
Quasi-static spherical shell model Semi analytical solution
Another way of assessing pore collapse mechanics is through a model on the mesoscale. Carroll & Holt (C&H) [2] used a spherical shell model. It is named after them, although they were not the first to use it. They developed a quasi-static solution and a dynamic solution, but assumed an incompressible matrix.
We develop similar solutions, and we take density changes into account. Our equations don’t look identical to those of C&H.
There are 3 stages as function of the boundary pressure Pb
: 1. Elastic, 2. Elastic-plastic and 3. fully plastic.
The elastic stage ends when:
a=inner boundary
b=outer boundary
12 March 2010Yehuda Partom13
At the elastic-plastic stage there are 4 unknowns: a, b, Pb
and the elastic-plastic boundary radius c. If one of them is specified, the others can be determined. It is easiest to specify a. Doing that we get 3 equations with 3 unknowns. The equations express: 1. Equation for b from the elastic field solution. 2. Continuity of σr
across the elastic-plastic boundary. 3. mass conservation. Density changes are included in the third equation by assuming:
The 3 equations are:
To solve these equations we differentiate them with respect to a

12 March 2010Yehuda Partom14
If and when c reaches the outer boundary (c=b) we enter the fully plastic stage. We have 2 equations: Pb
=σr
These can be solved directly by first eliminating .
In Figs. 4 we show results of an example for porous SS with 5 initial porosities φ0
=20%, 10%, 1%, 0.1%, 0.01%. In all the calculations b0
=1mm and a0
In Figs. 5 we show the Pb
(φ) curves during the pore collapse.
In Fig. 6 we show the Pb
(φ) curve when a becomes less then 0.0001 mm.
We see from the figures that:

When φ0

<1%,
the elastic plastic boundary approaches the outer boundary, but then turns around and goes back.
3 0
3 0
When φ0
is very small, the elastic-plastic boundary stays close to the inner boundary, and the pore closure pressure is finite and tends to 2/3Y, as seen from Fig. 6.
0 0.2 0.4 0.6 0.8 1 1.2 0
100
200
300
400
500
600
700
100
200
300
400
500
600
500
1000
1500
2000
200
400
600
800
100
200
300
400
500
Phi=.01% .1% 1% 10% 20%
P re
ss ur
e (G
P re
ss ur
e (G
P a)
O ut
si de
p re
ss ur
e w
he n
a b
ec om
Fig. 6
It provides a check to the semi-analytical solution.
It makes it possible to include more general elasto-plastic, visco-plastic and failure behavior.
The solution details are:
• For each integration step specify the displacement of the inner
boundary Δa.
.

Unknowns are determined from equilibrium equations for the staggered cells, which are:
• Using finite differences we get the system of equations:

scheme. For any approximation:
12 March 2010Yehuda Partom18
• Corrections to the unknowns are obtained by solving the linear system:
•The partial derivatives are determined by numerical differentiation. The system is tri-diagonal, but because u0
is given, it can be solved recursively in one sweep.
In Fig. 7 we compare with the semi-analytical solution for an initial porosity of 20%. In the numerical solution we let the material fail (lose its strength) linearly between effective plastic strain of 0.3 and 1.0.
ib b
i i
Semi analitical Numerical
Dynamic spherical shell model Semi analytical solution Without density changes
Mass conservation equation is:
Integrating with respect to r we get:
The momentum equation is:
Also, we approximate the stress deviator by its average as:
and check that:
from a to b we get:
If Pb
is given we get from this two simultaneous first order ODEs:
which can be integrated numerically.
v& ( ) 4
ab abG2G2 0000
12 March 2010Yehuda Partom21
In Fig. 8 we show an example of results using these equations. Again, it is a SS shell with 20% porosity and Pb
=20GPa.
0
0.2
0.4
0.6
0.8
1
1.2
a b
S he
ll ra
di us
(m m
Time (microsec)
Phi=20%
Fig. 8
We see from Fig. 8 that towards closure, the inner boundary velocity becomes extremely fast, and will probably get unstable.
We computed closure time as function of Pb
. We show the results in Fig. 9.
12 March 2010Yehuda Partom22
We see from Fig. 9 that for Pb
<1GPa the cavity does not close completely. This is different from the quasi-static solution. Also, we don’t get an elastic-
plastic stage, as we consider only averages of the shear stress components.
Including density changes
Using a similar approach, we’re able to consider average density changes. The mass conservation equation is then:
0
0.5
1
1.5
2
2.5
3
C lo
su re
ti m
e (m
ic ro
se c)
r v sr
For a constant Pb
the mass conservation equation is the same as before, and we may proceed as before (ignoring the small influence of the changing of s in the elastic region).
In Fig. 9 we show the porosity history for the same problem as before, and compare it to the result from the constant density run.
( )3 0
3 0
No density change With density change
P or
os ity
Time (microsec)
Phi=20%
Fig. 9
We see from Fig. 9 that the influence of density change is small, and that it slows the compaction process.
If Pb
=Pb
(t), the system of equations gets extremely complicated. We therefore chose not to work with these equations. Instead we approximate Pb
(t) by a staircase curve so that for each time step we have a constant Pb
. The error introduced can be checked by changing the integration time step.
12 March 2010Yehuda Partom25
Implementing in a hydro-code
( )
( )
Entering the material-energy stage, Vnew
for each computational cell at each time step is known, so that:
t VVV oldnew
=&
Using this with the previous shell model equations, and identifying the matrix pressure and density with the average shell model pressure and density, we have:
12 March 2010Yehuda Partom26
+=
&
&&
In Figs. 10 and 11 we compare results of a planar shock run with
the dynamic shell model to that with the quasi-static shell model.
0
5
10
15
20
25
Quasi-static shell model Dynamic shell model
P re
ss ur
e (G
P a)
Time (microsec)
P re
ss ur
e (G
P a)
Fig. 10 Fig. 11
12 March 2010Yehuda Partom27

For the quasi-static model the pores close at a relatively low pressure, while
for the dynamic model they close along the whole pressure range.
• For the dynamic model there is no elastic precursor.

For the quasi-static model the shock is sharp, while for the dynamic model the shock is smeared, like for a visco-plastic material.
Dynamic overstress model
For dynamic problems that have an equilibrium or quasi-static solution, the system usually tends towards this solution at a certain rate.
Let the quasi-static solution be:
( )Pqs =
12 March 2010Yehuda Partom28
then, at any stage during the pore closure process we have by the overstress approach:
and the simplest form of this relation is:
where the coefficient A may be calibrated from tests. Combining this with the equation that we had before:
we get a system of two first order ODEs to integrate for each cell at each time step as before.
In Figs. 12 and 13 we show examples of such simulations with different values of A: 0.01 and 0.02 (GPa μs)-1.
( )( )−= qsPPF&
∂∂ ∂∂
0.01 1/(GPa microsec) 0.02 1/(GPa microsec)
Pr es
su re
(G Pa
Pr es
su re
(G Pa
Fig. 12 Fig. 13
We see from Figs. 12 and 13 that the rate coefficient determines
the precursor level and the rise time. The P(V) curve is similar to that of the dynamic shell model, except for the precursor.
12 March 2010Yehuda Partom30
Summary Modeling compaction of porous materials started with the pioneering works of Herrmann and Carroll & Holt in the sixties and seventies. Interest in the subject increased when explosive compaction became a viable technology. Never the less, the material models haven’t changed much.
We present a survey of these models. They are based mainly on Herrmann’s EOS and on Carroll & Holts spherical shell model. The examples we show are our own contribution, and the detailed equations are sometimes different from those in the original papers.
The subject is still open to more research because:
• A spherical shell does not represent all possible geometries.
• The models are mainly for ductile materials.
• Collapse under pressure + shear could give different results.
• The size distribution of pores could have an effect.
Slide Number 1
Slide Number 2
Slide Number 3
Slide Number 4
Slide Number 5
Slide Number 6
Slide Number 7
Slide Number 8
Slide Number 9
Slide Number 10
Slide Number 11
Slide Number 12
Slide Number 13
Slide Number 14
Slide Number 15
Slide Number 16
Slide Number 17
Slide Number 18
Slide Number 19
Slide Number 20
Slide Number 21
Slide Number 22
Slide Number 23
Slide Number 24
Slide Number 25
Slide Number 26
Slide Number 27
Slide Number 28
Slide Number 29
Slide Number 30